  Lightweight refractory high-entropy alloy coatings (RHEAcs) of
NbxMo$_{0.5}$Ti$_{1.5}$Ta$_{0.2}$Cr (where $x=$ 1, 1.3, 1.5, and 2) were
fabricated on the surface of 316L stainless steel using laser cladding (LC)
technology. A comprehensive study was conducted to elucidate the effect of Nb
content on the microstructure, microhardness and wear resistance of
NbxMo$_{0.5}$Ti$_{1.5}$Ta$_{0.2}$Cr RHEAcs before and after annealing at 900
for 10 h. The results show that the grains are gradually refined with the
increase of Nb content. The coating consists mainly of a body-centered cubic
(BCC) solid solution, C15-Laves phase, and a small amount of hexagonal
close-packed (HCP) solid solution containing Ti. The microhardness of RHEAcs is
significantly higher compared to the base material. Notably, at Nb1.3, due to
the influence of lattice dislocations, the microhardness reaches a peak of
1066.5 HV, which is about 7.11 times higher than that of the base material. On
the contrary, at Nb$_2$, the microhardness is at its lowest point, averaging
709.31 HV, but 4.72 times that of the base material. After annealing, an
increase in microhardness is observed at all Nb concentrations, up to 31.2% at
Nb$_2$. Before annealing, the wear resistance of RHEAcs was slightly better
than that of 316L stainless steel at different Nb contents. However, after
annealing, the coefficient of friction (COF) and wear rate of the coatings are
lower than those of annealed 316L stainless steel, highlighting their excellent
wear resistance. It is noteworthy that the loss of wear properties after
annealing at Nb1 is at a minimum, obtaining the most balanced wear resistance
before and after annealing. The enhanced wear resistance after annealing can be
attributed to the presence of ultra-fine grain oxide friction layers, mainly
composed of TiO2 and Ta2O5 . The main mode of wear is oxidative wear, with a
small amount of wear from abrasive wear.
